Two excellent phase-matchable infrared nonlinear-optical materials based on the 3D diamond-like frameworks: RbGaSn2Se6 and RbInSn2Se6
Lin, Hua; Chen, Hong; Zheng, Yu-Jun; Yu, Ju-Song; Wu, Xin-Tao; Wu, Li-Ming; Dalton Trans.  (2017) –; doi:10.1039/C7DT01384A

data_7042981
_publ_section_title
;
 Two excellent phase-matchable infrared nonlinear-optical materials based
 on the 3D diamond-like frameworks: RbGaSn2Se6 and RbInSn2Se6
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT01384A
_journal_year                    2017
_chemical_formula_moiety         'In Rb Se6 Sn2'
_chemical_formula_sum            'In Rb Se6 Sn2'
_chemical_formula_weight         911.43
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           146
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3'
_symmetry_space_group_name_H-M   'R 3 :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2016-09-17 deposited with the CCDC.
2017-05-10 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   10.6044(8)
_cell_length_b                   10.6044(8)
_cell_length_c                   9.660(2)
_cell_measurement_reflns_used    1003
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4046
_cell_measurement_theta_min      3.0607
_cell_volume                     940.8(2)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2007)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  Mercury70
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0326
_diffrn_reflns_av_sigmaI/netI    0.0500
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            2300
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         3.06
_exptl_absorpt_coefficient_mu    26.982
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6240
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Red
_exptl_crystal_density_diffrn    4.826
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             1170
_exptl_crystal_size_max          0.2000
_exptl_crystal_size_mid          0.1700
_exptl_crystal_size_min          0.1200
_refine_diff_density_max         2.145
_refine_diff_density_min         -1.010
_refine_diff_density_rms         0.234
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.000(18)
_refine_ls_extinction_coef       0.00105(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_matrix_type           full
_refine_ls_number_parameters     33
_refine_ls_number_reflns         941
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.015
_refine_ls_R_factor_all          0.0274
_refine_ls_R_factor_gt           0.0254
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0118P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0483
_refine_ls_wR_factor_ref         0.0487
_reflns_number_gt                879
_reflns_number_total             941
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c7dt01384a2.cif
_cod_data_source_block           RbInSn2Se6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        940.7(2)
_cod_original_sg_symbol_H-M      R3
_cod_database_code               7042981